Download presentation

Presentation is loading. Please wait.

Published byGuillermo Murfin Modified over 3 years ago

1
1 CH-3 Energetic of fracture HUMBERT Laurent Thursday, march 11th 2010 laurent.humbert@epfl.ch laurent.humbert@ecp.fr

2
2 FRACTURE MECHANICS PROJECTS Group 1: Experimental project #1 Berglund Niklas Fogelfors Oscar Tunçer Gözde Group 2: Experimental project #2 Farmand Ashtiani Ebrahim Khoushabi Azadeh Group 3: Numerical project #3 Baader Jakob Bernet Adeline Uriarte Amaia RESPONSIBLES Laurent HUMBERTROOM ME C1 365 Samuel STUTZ ROOM ME C1 375 (group 2)

3
3 SESSIONS S1 Thursday, March 11 th 10h-12h group1 and 3 Friday, March 12 th 10h-12hgroup2 S2 Thursday, March 18 th 10h-12h group1 and 3 Friday, March 19 th 10h-12hgroup2 S3 Thursday, March 25 th 10h-12h group1 and 3 Friday, March 26 th 10h-12hgroup2 S4 Thursday, April 1 st 10h-12h group1 and 3 ? Friday, April 2 nd 10h-12hgroup2Good Friday S5 Thursday, April 15 th 10h-12h group1 and 3 Friday, April 16 th 10h-12hgroup2 S6 Thursday, April 22 nd 10h-12h group1 and 3 Friday, April 23 rd 10h-12hgroup2 S7 Thursday, April 29 th 10h-12h group1 and 3 Friday, April 30 th 10h-12hgroup2 S8 Thursday, May 6 th 10h-12h group1 and 3 Friday, May 7 th 10h-12hgroup2 S9 ? Thursday, May 13 th 10h-12h group1 and 3Ascension Day Friday, May 14 th 10h-12hgroup2 S10 Thursday, May 20 th 10h-12h group1 and 3 Friday, May 21 st 10h-12hgroup2 S11 Thursday, May 27 th 10h-12h groups 1, 2 and 3 Oral presentation Proposed work schedule...

4
4 3.1 Theoretical strength (recalls) Ideal crystal structure Equilibrium at inter-atomic distance a=a 0 Atomic scale Bond energy where l assumed to be approximately equal to twice the atomic spacing a 0 P = applied force Force-displacement relationship idealized as one half of the period of the sine wave Cohesive force P c Derivative of the potential energy interaction ° Lennard-Jones potential

5
5 - Lattice deformation: : critical stress (theoretical strength) Approximate Stress-strain relationship: - Dividing P by the number of bonds per unit area, - Assuming small strains (linear elastic), expanding the sin function in Taylor series: Young’s modulus:

6
6 And by taking, From the definition of the Young’s modulus : with more accurate calculations Introducing the surface energy : Surface energy of a solid = energy it costs to make it 2 new surfaces →

7
7 In reality : In practice, real materials do not achieve the ideal value Why ? Because all crystals contain defects : Such as vacancies, dislocations, imperfect grain boundaries depending on the environmental conditions

8
8 3.2 Griffith’s analysis of strength Stresses concentration appears in holes, slots, threads and huge change in section c : characteristic dimension associated with the defect → lower the global strength by magnifying the stress locally

9
9 Maximum local stress ? : minimum radius of curvature : stress concentration factor (dimensionless !) for tension for torsion and bending S 0 : nominal section Equation inexact but adequate working approximation for many design problems →

10
10 Examples : Circular hole of radius R in a large plate loaded in tension Local yielding occurs when ! Elliptical cavity (semi-axes a > b) traversing a plate loaded in tension R a b Result given by Inglis (1913)

11
11 Cracked material Cracks highly concentrate stress ! a

12
12 The engineering problem of a crack in a structure

13
13 Non uniform local stress : Cracks are sharp : - previous equation for holes, notches of finite radius of curvature not relevant here ! - their radius at the crack tip are essentially zero rises deeply at the crack tip With the minimum radius at crack tip Assuming failure when remote stress at failure → rough estimate : continuum approach of Inglis not valid at the atomic level

14
14 Griffith energy balance: Slender ellipse Total energy of the plate : : potential energy = strain energy U - work of external forces F : work required to create two new surfaces Griffith energy balance (equilibrium) : for an increment in the crack area dA B = Through crack in a plate of thickness B model based on a global energy approach

15
15 For the cracked plate configuration (plane stress conditions), Moreover with a constant thickness B and a through crack of length 2a : surface energy per unit area of the material Crack area = projected area of the crack = 2aB (here) Surface area = two matching surfaces = 4aB

16
16 Solving for a, equilibrium Energy crack length a

17
17 Solving for the stress : Type of equilibrium ? → sign of the second derivative of the energy → stable or unstable propagation Always unstable configuration ! fracture stress

18
18 Griffith approach applicable to other crack configurations : Ex: penny-shaped crack configuration Fracture stress : : Poisson’s ratio E : Young’s modulus a circular crack of radius a Remarks :

19
19 plastic work per unit area of surface created Large underestimation of the fracture strength for metals : → modified Griffith equation for materials that exhibit some plastic deformation (Irwin and Orowan) account for additional energy dissipation (e.g. dislocation motion) only valid for brittle solids (e.g. glass) → total energy of broken bonds in a unit area

20
20 General effect of temperature on the fracture energy of structural metals : Generalization for any type of energy dissipation : w f : fracture energy Limited to elastic global behavior (because of P ) and w f assumed to be constant ! → plastic, viscoelastic, viscoplastic effects

21
21 The force P does no work during a virtual crack increment : Glass wedge Strain energy : calculated by considering the thin layer as a cantilever beam ( of unit thickness, B=1) 3.3 Obreimoff’s experiment

22
22 Thus, Always stable configuration !

23
23 Cracked specimen under load : 3.4 Energy analysis – compliance method Potential energy : Total energy : Work F done by the applied forces ? Linear elastic behaviour : U ?

24
24 Compliance : Strain energy expressed by From the linear law, Clearly, Total energy (with unit thickness B=1) Crack propagation when Sign of Positive : stable propagation Negative : unstable propagation Note that when W s is a linear function of a

25
25 Energy release rate (ERR): By definition (Irwin 1956), Crack extension occurs when : Stability of the crack growth ? Stable crack propagation (controllable manner) Unstable crack propagation (uncontrollable manner) Ex : For the plate of with a center crack of length 2a Always unstable ! “crack driving force”

26
26 ERR under constant load : B Thus, Graphical interpretation : O D E

27
27 Expression with the compliance C : By reporting in the expression of G, one has differencing with respect to a, P constant : constant :

28
28 ERR under constant displacement Thus, Becauseand expression of G at constant load recovered ! Graphical interpretation : O A C Difference with load control negligible

29
29 Generalization : O a a +da P : possible relationship between the load P and the displacement D for a moving crack Identification of the crack driving force G A B C D E Thus, Having measured and knowing the loading curves for neighbouring crack areas, the development of the ERR can be followed

30
30 Example : Double Cantilever Beam (DCB) Double cantilever beam specimen at fixed load (a) or fixed grips (b) (a) (b)

31
31 Cracked structure with a finite system compliance : d and G are assumed to depend only of Structure held at a fixed remote displacement Differentiating,(1) Dividing by dA and fixing D, (2) (1) + (2) implies cf Anderson’s book

Similar presentations

Presentation is loading. Please wait....

OK

CH-4 Plane problems in linear isotropic elasticity

CH-4 Plane problems in linear isotropic elasticity

© 2018 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on sources of energy for class 8th maths Ppt on morphology of flowering plants for class 11 Ppt on accounting standards 19 Ppt on urbanization and environment Ppt on global marketing management Ppt on steve jobs biography for children Convert word doc to ppt online reader Download ppt on types of houses Free ppt on power quality Ppt on paintings and photographs related to colonial period dates